week ending 6 DECEMBER 2013

PHYSICAL REVIEW LETTERS

Coupling Light into Graphene Plasmons through Surface Acoustic Waves Ju¨rgen Schiefele,1,* Jorge Pedro´s,2,3,† Fernando Sols,1,3 Fernando Calle,2,3 and Francisco Guinea4 1

Departamento de Fı´sica de Materiales, Universidad Complutense de Madrid, E-28040 Madrid, Spain Instituto de Sistemas Optoelectro´nicos y Microtecnologı´a, Universidad Polite´cnica de Madrid, E-28040 Madrid, Spain 3 Campus de Excelencia Internacional, Campus Moncloa UCM-UPM, E-28040 Madrid, Spain 4 Instituto de Ciencia de Materiales de Madrid, CSIC, E-28049 Madrid, Spain (Received 3 September 2013; published 5 December 2013)

2

We propose a scheme for coupling laser light into graphene plasmons with the help of electrically generated surface acoustic waves. The surface acoustic wave forms a diffraction grating which allows us to excite the long lived phononlike branch of the hybridized graphene plasmon-phonon dispersion with infrared laser light. Our approach avoids patterning the graphene sheet, does not rely on complicated optical near-field techniques, and allows us to electrically switch the coupling between far-field radiation and propagating graphene plasmons. DOI: 10.1103/PhysRevLett.111.237405

PACS numbers: 78.67.Wj, 73.20.Mf, 77.65.Dq

Surface plasmon polaritons (hereafter called plasmons) are electromagnetic waves that are confined to the interface between two materials and accompanied by collective oscillations of surface charges [1]. The strong spatial confinement of the electromagnetic field and its coupling to charge carriers allow for the manipulation of light at subwavelength scales—beyond the diffraction limit of classical optics—which opens the possibility to integrate electronics and optics at the nanoscale. Further promising plasmonic applications include single molecule detection, metamaterials, and light harvesting [2]. Graphene, a single layer of carbon atoms arranged in a honeycomb lattice [3], forms a pure two-dimensional electron gas that supports plasmons in a broad frequency range from the midinfrared to the terahertz domain [4–6]. Unlike conventional plasmons in noble metals, graphene plasmons can be tuned in situ through the modulation of the carrier density by electrostatic gating. For long wavelengths k kF , the plasmon wave vector in graphene on a (nonpolar) dielectric substrate is approximately given by [7] k¼

!p Ep eff ; c EF 2fs

(1)

where Ep ¼ @!p is the plasmon energy, eff ¼ ð1 þ 1Þ=2 the effective average over the dielectric constants ofﬃ substrate and air, and the Fermi energy EF ¼ pﬃﬃﬃﬃﬃﬃ @vF n can be adjusted with the carrier density n. The strong field concentration typical for plasmon excitations results in a large wave vector mismatch k !p =c, which is revealed by the small magnitude of the fine-structure constant fs ’ 1=137 in Eq. (1). Therefore, the excitation of plasmons with free-space radiation requires diffraction of the incident light at structures with dimensions smaller than 2c=!p . In the experiments realized so far, grapheneplasmon laser coupling required either complex near-field techniques [8,9] or the patterning of micro- or nanoscale arrays for far-field coupling [10–13], where edge scattering 0031-9007=13=111(23)=237405(5)

reduces the plasmon lifetime. In this work, we propose a scheme for converting far-field radiation into graphene plasmons by deforming the graphene sheet with a surface acoustic wave (SAW) and thus forming a tunable optical grating without the need of any patterning. Our calculation shows that long-lived midinfrared plasmons, hybridized with surface phonons in the supporting piezoelectric materials, are excited with good efficiencies. Figure 1 shows a sketch of the proposed device, where a high-frequency signal applied to an interdigital transducer (IDT) on a piezoelectric film generates a Rayleigh-type SAW propagating in the x direction. The graphene sheet is periodically deformed in the x-z plane by the strain field of the wave. Thus, a propagating grating with an adjustable amplitude up to a few nanometers and a period in the submicron range can be formed. By diffraction on the grating, incident TM polarized laser light (that is, with its E field polarized in the x-z-plane) can overcome the momentum mismatch and excite plasmons in the graphene sheet. AlN and ZnO have been selected as piezoelectric materials since they present large electromechanical coupling coefficients and Laser IDT

z

θ

Graphene SAW

x

Piezoelectric film Substrate

Gate

FIG. 1. Sketch of the device. A high-frequency signal applied to an interdigital transducer (IDT) on a piezoelectric film generates a surface acoustic wave (SAW) propagating in the x direction. The graphene sheet is deformed by the SAW, the periodic deformation acting as a refraction grid for the incident laser beam. A back gate allows tuning the Fermi energy of graphene.

237405-1

Ó 2013 American Physical Society

PRL 111, 237405 (2013)

their high-quality thin films can be deposited by sputtering on a variety of substrates [14,15]. Submicron IDTs on these materials allow SAWs operating well above 10 GHz [15,16]. A back gate, deposited on the substrate before sputtering the film, allows us to tune the graphene plasmon dispersion in and out of resonance with the laser. The material underneath the graphene influences its electronic properties, as the charge carriers in graphene couple to the long-range electric fields generated by optically active phonon modes in the surrounding material [17]. This mechanism is known to influence charge transport and drag effects in graphene [18–20], as well as to alter the dispersion of graphene plasmons on polar substrates [12,21]. Piezoelectric materials are polar by definition. For the dielectric function of the piezoelectric film, an oscillator model is assumed: ð!Þ ¼ 1 þ ð0 1 Þ

!2TO ; !2TO !2 þ 2i!

(2)

where !TO denotes the frequency of the transverse optical phonon, its damping rate, and 0 and 1 the static and high-frequency dielectric constants, respectively. The coupling strength between carriers in the graphene sheet and polar surface phonons (with frequency !sp ) located at the surface of the piezoelectric film is given by [17,19,22] qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ (3) MðkÞ ¼ gekz0 cfs @2 !sp =k: Here, k ¼ ðkx ; ky Þ is the surface-phonon wave vector, the coupling constant g ¼ fð0 1 Þ=½ð1 þ 1 Þð1 þ 0 Þg1=2 , z0 > 0 denotes the graphene-substrate separation, and !sp is the solution of the equation 1 þ ð!Þ ¼ 0. As the wave vector range of interest here is k 107 m1 and z0 3 A for the common substrate materials, the exponential factor has been set to unity in the following. Apart from the coupling to substrate phonons, graphene electrons also couple to in-plane optical and out-of-plane (flexural) phonon modes in the graphene sheet itself. While the former would play a role only at plasmon energies above 200 meV [12], which are out of our parameter range, the latter process is strongly suppressed in substrate supported graphene sheets [23,24], and in the following, we neglect both of these scattering mechanisms. Because of the coupling MðkÞ, charge carriers in the graphene sheet can interact by exchange of surface phonons, which leads to the potential [21] V!sp ðk; !; sp Þ ¼ jMðkÞj2 G!sp ð!; sp Þ;

(4)

where the lifetime of the surface phonon sp enters the phonon propagator G!sp ð!; sp Þ ¼

week ending 6 DECEMBER 2013

PHYSICAL REVIEW LETTERS

2!sp : @½ð! þ i=sp Þ2 !2sp

(5)

For AlN (0 ¼ 7:37, 1 ¼ 3:93) we obtain g ¼ 0:289 and @!sp ¼ 106 meV, for ZnO (0 ¼ 7:46, 1 ¼ 3:61), g ¼ 0:314 and @!sp ¼ 68 meV [25]. The total effective carrier interaction results from Coulomb interaction VC ¼ e2 =ð2kvac eff Þ [with vac ¼ e2 =ð4@fs cÞ the permittivity of free space] and phonon exchange. Within the random phase approximation (RPA), it reads [21,28] eff VRPA ¼

VC þ V!sp 1 ðVC þ V!sp Þð0Þ

¼

VC ; RPA

(6)

where ð0Þ denotes the polarizability of graphene [29,30] which depends parametrically on the electron relaxation time e [31]. The last equality in Eq. (6) defines the total dielectric screening function RPA ðk; !Þ. The plasmon dispersion can be obtained by (numerically) solving the equation RPA ðk; !Þ ¼ 0, which depends on the dielectric function of the piezoelectric film via V!sp in Eq. (6). An approximate analytical expression can be obtained from Eq. (6) by setting the scattering times sp , e ! 1 and ð0Þ EF k2 =ð@2 !2 Þ, which is valid for ! > vF k and EF @!. Solving for the zeros of RPA yields the two solutions !2p ðkÞ

qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 ¼ ½!2sp þ !2p ð!2sp þ !2p Þ2 4!2p !2sp ð1 2g2 eff Þ; 2 (7)

where !p ðkÞ is given by Eq. (1). The two branches !p shown as white curves in Figs. 2(a) and 2(c) describe coupled excitations involving both collective electronic and lattice oscillations. In the limit g ! 0 of vanishing substrate coupling, !pþ ! !sp and !p ! !p , and the unhybridized system is recovered. The plasmon lifetimes p shown in Figs. 2(b) and 2(d)— of the order of 1013 s—are obtained by solving the equation RPA ¼ 0 for the imaginary part of the plasmon frequency. As a function of frequency, they vary between the boundaries set by the surface-phonon damping sp , assumed to be 1 ps as reported in Ref. [12], and the electron relaxation time of graphene, e ¼ EF =v2F , where is the carrier mobility. For low k values, the !pþ branch is dominated by sp rather than e , allowing us to excite relatively long-lived plasmons. In the limit k ! 0, p ¼ sp . Conversely, the !p branch shows a stronger damping, due to the larger influence of e . Plasmon excitation manifests itself in enhanced light absorption. The transmittance and reflectance of graphene on a dielectric substrate can be calculated from the Fresnel reflection and transmission coefficients [32]

237405-2

PRL 111, 237405 (2013)

Figs. 2(a) and 2(c)] displays peak values along the two branches !p of Eq. (7). Figure 3(a) shows the transmittance through the air-graphene-AlN (red curve) and air-AlN (blue curve) interface in the frequency range @! ¼ 0-0:2 eV for normal incident light. A region of low transmittance is observed between the transverse and longitudinal optical phonon frequencies of AlN. In the presence of graphene, the transmittance at low frequencies is reduced due to the Drude response. Within the frequency range of the !pþ branch, both AlN and graphene-AlN are seen to be almost transparent. In the presence of the SAW, the transmittance changes, because a TM polarized laser beam can overcome the momentum mismatch and excite plasmons: the SAW imposes a sinusoidal deformation of wavelength g and amplitude on the graphene. This corrugation works like a diffraction grating that scatters incident light with wave vector (kk0 , kz0 ) into the various diffraction orders (kkm , kzm ), with

0.10

= 0.25 m

Graphene/AlN

g

=1 m

sp

=1 m

g

[eV]

0.15

g

0.05

(b)

(a)

0.00

Graphene/ZnO = 0.25 m

[eV]

g

=1 m

0.15

0.10

g

sp

0.05

0.00

(d) 0.8

(c)

0

1

k [m-1 x 107]

2

0.4 p

[ps]

FIG. 2. (a), (c) Plasmon dispersion for graphene on AlN and on ZnO, respectively. The two hybridized plasmon branches are well described by the asymptotic expressions !p ðkÞ of Eq. (7) (white curves). The contour plot shows the imaginary part of the reflection coefficient rTM ðk; !Þ; see Eq. (8a). Parameters are EF ¼ 0:4 eV and e ¼ 2 1013 s (corresponding to a mobility of 5000 cm2 V1 s1 ). The white triangular area indicates the region of high intraband loss, ! < vF k. (b), (d) Plasmon lifetime p along the two branches.

ð!Þkz k0z þ ð!Þkz k0z =ðvac !Þ ; (8a) ð!Þkz þ k0z þ ð!Þkz k0z =ðvac !Þ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 ð!Þkz TM ; (8b) t ðk; !Þ ¼ ð!Þkz þ k0z þ ð!Þkz k0z =ðvac !Þ k k0z !ð!Þ=ðc2 vac Þ rTE ðk; !Þ ¼ tTE 1 ¼ z ; (8c) kz þ k0z þ !ð!Þ=ðc2 vac Þ

rTM ðk; !Þ ¼

where TM and TE denote the polarization of the incident pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ beam, kz ¼ ð!=cÞ2 k2 and k0z ¼ ð!Þð!=cÞ2 k2 are the z components of the wave vector in air and in the substrate, respectively, and ð!Þ ¼

week ending 6 DECEMBER 2013

PHYSICAL REVIEW LETTERS

e2 EF i @2 ! þ i=e e2 i @! 2EF ð@! 2EF Þ þ log þ (9) [email protected] @! þ 2EF

is the conductivity of graphene at zero temperature [31], which yields a good approximation as long as T TF . In the nonretarded limit !=c k, the zeros of RPA are identical to the poles of rTM . Correspondingly, the absorption of light given by ImrTM [shown by the contour plots in

kkm ¼ ð!=cÞ sin þ m2=g ;

(10)

qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ kzm ¼ ð!=cÞ2 k2km ;

(11)

where denotes the angle of off-normal incidence and m is an integer. To excite plasmons, the frequency of the plasmon has to coincide with the laser frequency, and its k vector with one of the kkm , which in turn can be chosen by an appropriate SAW wavelength g [33]. The intensity of the diffracted light in mth order, normalized to the intensity of the incoming beam, is given by [34] 2 m 1 þ r ðmÞ : (12) I ¼ rJm ð2kz0 Þ 1 þ k r g zm

Here, r denotes, depending on the polarization of incident light, rTM ð!; kkm Þ or rTE ð!; kkm Þ [see Eqs. (8)]. As the corrugation amplitude achievable with SAWs is of the order of a few nanometers, kz0 1, and the relative intensities I ðmÞ are suppressed proportionally to the Bessel function jJm ð2kz0 Þj2 ’ ðkz0 Þ2m . The range of wave vectors in which plasmons can be excited is determined by g , i.e., by the period of the IDT. With electron-beam or nanoimprint lithography, periods of 0:25–1 m can be realized [14–16]. For normal incidence, kk1 then takes values between ð0:6–2:5Þ 107 m1 , as indicated by the vertical dotted lines in Figs. 2(a) and 2(c). For kk1 within this range and ! along the plasmon dispersion, kz1 is imaginary, and the electric field of the diffracted beam decays exponentially in the direction perpendicular to the surface. The transmittance T in the presence of a SAW (with g ¼ 0:25 m and EF ¼ 0:4 eV) is shown in Fig. 3(b) for TE and TM polarization (red and black curves, respectively). While the former does not deviate from the

237405-3

PRL 111, 237405 (2013) 1.0

1.00

Transmittance

AlN Graphene/AlN

60

Graphene/AlN TM =0 nm TE =4 nm TM =4 nm

0.970

0.5

Graphene/AlN TM =0 nm TM =4 nm

30 0.98

0.965

0 TO

0.0 0.0

1.5 1.0 0.5

(a)

LO

0.1

2.0

1-TTM( )/TTM(0) [%]

week ending 6 DECEMBER 2013

PHYSICAL REVIEW LETTERS

Graphene/AlN -1 [1013 Hz] e 0.25 0.5 0.4 eV 1

0.960

0.16

0.140

Graphene/AlN

0.2

EF = 0.2 eV

0.14

0.136

0.4 0.6 eV Graphene/AlN -1 [1013 Hz] e 0.25 0.4 eV 0.5 1

0.002

E F= 0.2 eV

0.12

(c) 0.140 0.96

0.136

0.004

0.6 eV

(d) 0.0

(b) 0.2

0

30 60

(e)

0.000 0.02

0.04

[eV]

0.06

[eV]

0.08

0.0

(f) 0.136

0.140

[eV]

FIG. 3 (color online). (a) Transmittance of AlN and graphene on AlN in the absence of surface corrugation, normal incident light. (b) Change in the transmittance of TM polarized light due to plasmon excitation in the presence of a SAW. SAW amplitude ¼ 4 nm and period g ¼ 0:25 m, graphene parameters EF and e as in Fig. 2. (c) Same as (b) for various angles of incidence . (d) Extinction spectrum of graphene on AlN in the presence of a SAW ( ¼ 4 nm and g ¼ 0:25 m) for different values of EF and e . Peaks are due to excitation of plasmons in the !pþ branch [see Eq. (7)]. (e) Same as (d) for excitation of plasmons in the !p branch, ¼ 4 nm and g ¼ 1 m. (f) Extinction spectrum corresponding to (c).

transmittance at an uncorrugated interface (black dashed curve), the latter displays a dip due to plasmon excitation in the !pþ branch. As the two plasmon branches get steeper with increasing EF , the plasmon resonance blueshifts. This is shown in the extinction spectra 1 T TM ðÞ=T TM ð0Þ of Figs. 3(d) and 3(e) for the !p branches, respectively. The height of the peaks can serve as a figure of merit for the efficiency of plasmon excitation. For fixed EF and g , it depends on the graphene quality through the electron relaxation time e . The solid, dashed, and dotted curves in Figs. 3(d) and 3(e) were obtained by setting 1 e to 0.25, 0.5, and 1 1013 Hz, respectively. The height of the resonance increases with e , as damping of the collective electron oscillations decreases. For @! * 0:6 eV, the plasmon resonance of the !p branch in Fig. 3(e) begins to merge with the phonon resonances of AlN [see Fig. 3(a)]. As the intensity of incident light diffracted to second order [m ¼ 2 in Eq. (12)] is smaller by a factor of 105 compared to the first order, extinction peaks due to the excitation of plasmons with wave vector kk2 are not visible on the scale of Figs. 3(d) and 3(e). The extinction spectra for graphene on ZnO are qualitatively similar to those shown for AlN, but allow us, due to the lower surface-phonon frequency, to excite !pþ plasmons with longer laser wavelengths (see Fig. 2(c)]. As !=c 2=g , the -dependent term in Eq. (10) shifts the plasmon resonance only slightly, as shown by the

transmittance and extinction spectra in Figs. 3(c) and 3(f). The strength of the resonance, however, is maximal for normal incident light, because only the x component of the electric field excites plasmons. Because of the 2 dependence in the diffraction intensity of Eq. (12), the achievable efficiency also depends strongly on the SAW amplitude. With the realistic value of 4 nm used in Fig. 3 [35], the predicted extinction values are comparable to those obtained in Ref. [12] with patterned graphene. However, exciting plasmons in an extended graphene sheet avoids plasmon damping due to edge scattering, which severely limits plasmon lifetimes in patterned graphene [12]. Moreover, the SAW-assisted plasmon generation mechanism in homogeneous graphene will permit us to design plasmonic devices using propagating plasmons, otherwise impeded in patterned graphene structures. We have demonstrated that SAWs can be used to generate a switchable refraction grid which couples laser light into the hybridized plasmon supported by graphene on piezoelectric materials like, for example, ZnO and AlN. The coupling to surface phonons shifts the low wave vector part of the graphene plasmon dispersion, which is virtually unaffected by intraband losses, upwards into the attractive midinfrared frequency range. Because of their relatively low damping in the vicinity of the surface-phonon frequency, these phononlike plasmon branches have a high potential for photonic applications.

237405-4

PRL 111, 237405 (2013)

PHYSICAL REVIEW LETTERS

The proposed scheme for plasmon excitation avoids the patterning of graphene, diminishing the edge scattering and generating propagating plasmons which could be used in future graphene-based plasmonic devices. Moreover, plasmons can be switched electrically, via the highfrequency signal at the IDT, whereas the plasmon resonance can be tuned via electrostatic gating. In addition, the IDT technology allows for many different plasmon functionalities. For example, curved IDTs can create interfering SAWs for plasmon focusing [36]. Thus, SAWs offer the possibility to tailor electrically switchable graphene-based metamaterials. We would like to thank Frank Koppens, Christopher Gaul, and Harald Haakh for helpful remarks. The authors acknowledge support from the Marie Curie ITN NanoCTM, the Campus de Excelencia Internacional (Campus Moncloa UCM-UPM), ERC Advanced Grant No. 290846, and MICINN (Spain) through Grants No. FIS2008-00124, No. FIS2010-21372, No. TEC201019511, and No. FIS2011-23713. Note added in proof.—After this Letter was accepted for publication, we became aware of related work reporting a different technique to excite graphene plasmons through excitation of elastic vibrations [37].

*[email protected] † [email protected] [1] S. A. Maier, Plasmonics: Fundamentals and Applications (Springer, New York, 2007). [2] A. Polman, Science 322, 868 (2008). [3] A. H. C. Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and A. K. Geim, Rev. Mod. Phys. 81, 109 (2009). [4] F. H. L. Koppens, D. E. Chang, and F. J. Garcia de Abajo, Nano Lett. 11, 3370 (2011). [5] A. N. Grigorenko, M. Polini, and K. S. Novoselov, Nat. Photonics 6, 749 (2012). [6] Y. V. Bludov, A. Ferreira, N. M. R. Peres, and M. I. Vasilevskiy, Int. J. Mod. Phys. B 27, 1341001 (2013). [7] This relation follows from a semiclassical (Drude) model for the graphene conductivity, which only takes into account the first term of Eq. (9) and neglects disorder, e ! 1. [8] J. Chen, M. Badioli, P. Alonso-Gonzalez, S. Thongrattanasiri, F. Huth, J. Osmond, M. Spasenovic, A. Centeno, A. Pesquera, P. Godignon et al., Nature (London) 487, 77 (2012). [9] Z. Fei, A. S. Rodin, G. O. Andreev, W. Bao, A. S. McLeod, M. Wagner, L. M. Zhang, Z. Zhao, M. Thiemens, G. Dominguez et al., Nature (London) 487, 82 (2012). [10] L. Ju, B. Geng, J. Horng, C. Girit, M. Martin, Z. Hao, H. A. Bechtel, X. Liang, A. Zettl, Y. R. Shen et al., Nat. Nanotechnol. 6, 630 (2011). [11] A. Y. Nikitin, F. Guinea, F. J. Garcı´a-Vidal, and L. Martı´nMoreno, Phys. Rev. B 84, 161407 (2011).

week ending 6 DECEMBER 2013

[12] H. Yan, T. Low, W. Zhu, Y. Wu, M. Freitag, X. Li, F. Guinea, P. Avouris, and F. Xia, Nat. Photonics 7, 394 (2013). [13] M. Freitag, T. Low, W. Zhu, H. Yan, F. Xia, and P. Avouris, Nat. Commun. 4, 1951 (2013). [14] J. Pedro´s, L. Garcı´a-Gancedo, C. J. B. Ford, J. P. Griffiths, G. A. C. Jones, and A. J. Flewitt, Appl. Phys. Lett. 102, 043507 (2013). [15] J. Rodrı´guez-Madrid, G. Iriarte, J. Pedro´s, O. Williams, D. Brink, and F. Calle, IEEE Electron Device Lett. 33, 495 (2012). [16] S. Bu¨yu¨kko¨se, B. Vratzov, D. Atac¸, J. van der Veen, P. V. Santos, and W. G. van der Wiel, Nanotechnology 23, 315303 (2012). [17] N. Mori and T. Ando, Phys. Rev. B 40, 6175 (1989). [18] J. Schiefele, F. Sols, and F. Guinea, Phys. Rev. B 85, 195420 (2012). [19] E. H. Hwang and S. Das Sarma, Phys. Rev. B 87, 115432 (2013). [20] B. Amorim, J. Schiefele, F. Sols, and F. Guinea, Phys. Rev. B 86, 125448 (2012). [21] E. H. Hwang, R. Sensarma, and S. D. Sarma, Phys. Rev. B 82, 195406 (2010). [22] S. Fratini and F. Guinea, Phys. Rev. B 77, 195415 (2008). [23] E. V. Castro, H. Ochoa, M. I. Katsnelson, R. V. Gorbachev, D. C. Elias, K. S. Novoselov, A. K. Geim, and F. Guinea, Phys. Rev. Lett. 105, 266601 (2010). [24] B. Amorim and F. Guinea, Phys. Rev. B 88, 115418 (2013). [25] Material parameters for AlN and ZnO are taken from Refs. [26,27], respectively. [26] M. Kazan, S. Pereira, M. R. Correia, and P. Masri, J. Appl. Phys. 106, 023523 (2009). [27] N. Ashkenov, B. N. Mbenkum, C. Bundesmann, V. Riede, M. Lorenz, D. Spemann, E. M. Kaidashev, A. Kasic, M. Schubert, M. Grundmann et al., J. Appl. Phys. 93, 126 (2003). [28] G. D. Mahan, Many-Particle Physics (Plenum, New York, 1981). [29] B. Wunsch, T. Stauber, F. Sols, and F. Guinea, New J. Phys. 8, 318 (2006). [30] E. H. Hwang and S. Das Sarma, Phys. Rev. B 75, 205418 (2007). [31] M. Jablan, H. Buljan, and M. Soljacˇic´, Phys. Rev. B 80, 245435 (2009). [32] R. Messina and P. Ben-Abdallah, Sci. Rep. 3, 1383 (2013). [33] C. Ruppert, J. Neumann, J. B. Kinzel, H. J. Krenner, A. Wixforth, and M. Betz, Phys. Rev. B 82, 081416 (2010). [34] E. C. Lean, in Progress in Optics, edited by E. Wolf (North-Holland, Amsterdam, 1973), Vol. XI, p. 123. [35] R. Shilton, M. K. Tan, L. Y. Yeo, and J. R. Friend, J. Appl. Phys. 104, 014910 (2008). [36] L. Yin, V. K. Vlasko-Vlasov, J. Pearson, J. M. Hiller, J. Hua, U. Welp, D. E. Brown, and C. W. Kimball, Nano Lett. 5, 1399 (2005). [37] M. Farhat, S. Guenneau, and H. Bag˘c, preceding Letter, Phys. Rev. Lett. 111, 237404 (2013).

237405-5